Presentation on theme: "1 Tire repair procedures This presentation has been prepared from copyrighted materials from REMA TIP TOP / North America and is reproduced with their."— Presentation transcript:
1 Tire repair procedures This presentation has been prepared from copyrighted materials from REMA TIP TOP / North America and is reproduced with their permission
2 Warning! Always demount the tire from the wheel and complete a thorough tire and wheel inspection prior to returning the components to service.
19 Step 1.6 Inspect the injury with an awl, probing the injury to determine the extent of the damage and determine the inclination angle of the injury channel. Dipping the awl into BL-8F Special Blue Cement before probing the injury channel serves as a lubricant, allowing easier insertion of the awl to inspect the injury. Inspect the tire for any other damage. (See “WARNING”, ‘PRECAUTIONS”, GENERAL SAFETY INSTRUCTIONS” and “NON-REPAIRABLE TIRE CONDITIONS” sections earlier.
23 Step 3.1 Determine the correct size carbide cutter from the NAIL HOLE REPAIR CHART. Use a low speed tool (not to exceed 1200 rpm) to drill the injury from the inside out two or three times first and then from the outside in once or twice. Use full strokes with the carbide cutter, completely removing the cutter from the tire with each stroke.
26 Step 5.1 Center the repair unit over the injury and outline an area larger than the unit, so buffing will not remove the crayon marks. If the repair unit has bead arrows, make sure the arrows are pointing to the bead.
27 Step 5.2 Note: If during the buffing process the Radial Plies (or body plies) are damaged or exposed, the tire should be replaced. Lightly buff the repair area using a low speed (<5,000 RPM) air or electric buffing tool with a clean buffing rasp, 18 to 36 grit and remove all vent lines until you get a completely smooth surface. Continue lightly buffing the repair area to a smooth velvety finish (RMA Buff Texture 1 or 2) by putting slight pressure on the buffing tool and keeping it in constant movement.
28 Step 6.1 Clean the buffed area with a 6014 Brass Brush by brushing the area several times in one direction. Avoid brushing the non- buffed areas where there are contaminants that could be pulled into the freshly buffed area. Use a brush that is designated only for tire repair and not used for anything else. This will help avoid contaminates in the buffed area.
29 Step 6.2 Use a vacuum to remove all debris from the inside of the tire. Do not touch the buffed area with the tip of the vacuum cleaner to avoid contamination. Always remove buffing dust with the use of a brass brush and vacuum. Never use compressed air. Do not use Pre-Buff Cleaner on the buffed texture after you have buffed to avoid leaving residues which reduce adhesion.
31 Step 7.2 Apply a thin, even coat of BL-8F Special Blue Cement to the buffed area of the tire innerliner using a clean brush. Using a swirling motion to apply the cement, as this will aid in the drying process as well as assure a thin, even coat. Completely cover the buffed area with cement to assure a good bond between the tire and the Repair Unit. Continue brushing and working the cement into the buffed area until the cement appears to dry. Do not go outside the buffed area (Contaminates the brush). Rotate the tire so that the cemented area is located between the 10 o’clock and 2 o’clock position. This will allow the solvent vapors, which are heavier than air, to “fall” away from the cemented inner liner.
32 Step 7.2 Check the cement for dryness by touching the edge of the cemented area with the back of your finger. If the cement feels tacky, then it is dry. If it is not tacky, allow more drying time. Drying time depends on atmospheric conditions like heat and humidity. Hot temperature and dry humidity require longer drying time of the cement. If the cement is not completely dry, the repair unit will lift off or blister and cause a repair failure. Never use compressed air, hair driers, heat guns, etc to aid in the drying of the cement. Avoid any contamination on the bonding layer or the coat applied.
35 Step 7.6 After the repair unit is applied, stitch thoroughly from the center outwards. Always start stitching from the center outward to remove any trapped air that may be under the repair unit. Continue several times in different directions over the whole surface of the repair unit to make sure that it is completely stitched to the innerliner and that it adheres securely to the buffed surface area.
36 Step 8.1 Check the repair areas for defects. The finished repair should show no peeling or lifting at the edges, and should neatly cover the repair area. Apply a generous application of 76F Innerliner Repair Sealant to the entire over-buffed area and the edge of the repair unit. If a MINICOMBI has been used, Apply the Repair Sealant to the base of the MINICOMBI and any still exposed buffed areas.